| Sample no. | Composition (mol%) | Composition (mol%) | Density d (gcm-3) | Glass molar volume (V m) | Additive oxide volume (V o) | Volume deviation (V x) |
| Sample no. | Bi2O3              | B2O3               | Density d (gcm-3) | Glass molar volume (V m) | Additive oxide volume (V o) | Volume deviation (V x) |
| 1          | 20                 | 80                 | 4.457+-0.002      | 33.40                    | 41.07                       | -7.66                  |
| 2          | 25                 | 75                 | 4.815+-0.002      | 35.04                    | 41.78                       | -6.74                  |
| 3          | 30                 | 70                 | 5.470+-0.003      | 34.46                    | 42.48                       | -8.01                  |
| 4          | 33                 | 67                 | 5.636+-0.003      | 35.56                    | 42.91                       | -7.34                  |
| 5          | 37.5               | 62.5               | 6.006+-0.003      | 36.34                    | 43.54                       | -7.20                  |
| 6          | 40                 | 60                 | 6.246+-0.001      | 36.51                    | 43.89                       | -7.36                  |
| 7          | 41                 | 59                 | 6.359+-0.006      | 36.50                    | 44.03                       | -7.53                  |
| 8          | 42                 | 58                 | 6.389+-0.003      | 36.95                    | 44.17                       | -7.22                  |
| 9          | 47                 | 53                 | 6.737+-0.004      | 37.98                    | 44.88                       | -6.89                  |
| 10         | 50                 | 50                 | 6.874+-0.005      | 38.96                    | 45.30                       | -6.54                  |
| 11         | 53                 | 47                 | 7.074+-0.005      | 39.54                    | 45.73                       | -6.19                  |
| 12         | 55                 | 45                 | 7.214 +- 0.004    | 39.85                    | 46.01                       | -6.15                  |
| 13         | 60                 | 40                 | 7.550+-0.011      | 40.72                    | 46.71                       | -5.99                  |
| 14         | 66                 | 34                 | 7.765+-0.020      | 42.65                    | 47.56                       | -4.90                  |

Caption: Density, molar volume, additive oxide volume and volume deviations for bismuth borate glasses

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "1", "type": "Other"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "1"}
{"value": "80", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "1"}
{"value": "4.457", "type": "Other"}
{"value": "33.40", "type": "Other"}
{"value": "41.07", "type": "Other"}
{"value": "2", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "2"}
{"value": "75", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "2"}
{"value": "4.815", "type": "Other"}
{"value": "35.04", "type": "Other"}
{"value": "41.78", "type": "Other"}
{"value": "3", "type": "Other"}
{"value": "30", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "3"}
{"value": "70", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "3"}
{"value": "5.470", "type": "Other"}
{"value": "34.46", "type": "Other"}
{"value": "42.48", "type": "Other"}
{"value": "4", "type": "Other"}
{"value": "33", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "4"}
{"value": "67", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "4"}
{"value": "5.636", "type": "Other"}
{"value": "35.56", "type": "Other"}
{"value": "42.91", "type": "Other"}
{"value": "5", "type": "Other"}
{"value": "37.5", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "5"}
{"value": "62.5", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "5"}
{"value": "6.006", "type": "Other"}
{"value": "36.34", "type": "Other"}
{"value": "43.54", "type": "Other"}
{"value": "6", "type": "Other"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "6"}
{"value": "60", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "6"}
{"value": "6.246", "type": "Other"}
{"value": "36.51", "type": "Other"}
{"value": "43.89", "type": "Other"}
{"value": "7", "type": "Other"}
{"value": "41", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "7"}
{"value": "59", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "7"}
{"value": "6.359", "type": "Other"}
{"value": "36.50", "type": "Other"}
{"value": "44.03", "type": "Other"}
{"value": "8", "type": "Other"}
{"value": "42", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "8"}
{"value": "58", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "8"}
{"value": "6.389", "type": "Other"}
{"value": "36.95", "type": "Other"}
{"value": "44.17", "type": "Other"}
{"value": "9", "type": "Other"}
{"value": "47", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "9"}
{"value": "53", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "9"}
{"value": "6.737", "type": "Other"}
{"value": "37.98", "type": "Other"}
{"value": "44.88", "type": "Other"}
{"value": "10", "type": "Other"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "10"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "10"}
{"value": "6.874", "type": "Other"}
{"value": "38.96", "type": "Other"}
{"value": "45.30", "type": "Other"}
{"value": "11", "type": "Other"}
{"value": "53", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "11"}
{"value": "47", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "11"}
{"value": "7.074", "type": "Other"}
{"value": "39.54", "type": "Other"}
{"value": "45.73", "type": "Other"}
{"value": "12", "type": "Other"}
{"value": "55", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "12"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "12"}
{"value": "7.214", "type": "Other"}
{"value": "39.85", "type": "Other"}
{"value": "46.01", "type": "Other"}
{"value": "13", "type": "Other"}
{"value": "60", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "13"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "13"}
{"value": "7.550", "type": "Other"}
{"value": "40.72", "type": "Other"}
{"value": "46.71", "type": "Other"}
{"value": "14", "type": "Other"}
{"value": "66", "type": "Glass_Compound_Amount", "constituent": "Bi2O3", "unit": "mol", "material": "14"}
{"value": "34", "type": "Glass_Compound_Amount", "constituent": "B2O3", "unit": "mol", "material": "14"}
{"value": "7.765", "type": "Other"}
{"value": "42.65", "type": "Other"}
{"value": "47.56", "type": "Other"}